Nanoparticle are particles between 1 and 100 nanometres (nm) in size with a surrounding interfacial layer. The interfacial layer is an integral part of nanoscale matter, fundamentally affecting all of its properties. The interfacial layer typically consists of ions, inorganic and organic molecules. Organic molecules coating inorganic nanoparticles are known as stabilizers, capping and surface ligands, or passivating agents. In nanotechnology, a particle is defined as a small object that behaves as a whole unit with respect to its transport and properties. Particles are further classified according to diameter.
Note 2: The basis of the 100-nm limit is the fact that novel properties that
differentiate particles from the bulk material typically develop at a critical
length scale of under 100 nm.
Note 3: Because other phenomena (transparency or turbidity, ultrafiltration,
stable dispersion, etc.) that extend the upper limit are occasionally considered,
the use of the prefix nano is accepted for dimensions smaller than 500 nm,
provided reference to the definition is indicated.
According to ISO Technical Specification 80004, a nanoparticle is defined as a nano-object with all three external dimensions in the nanoscale, whose longest and shortest axes do not differ significantly, with a significant difference typically being a factor of at least 3. Nanoparticles can exhibit size-related properties significantly different from those of either fine particles or bulk materials.
Nanoclusters have at least one dimension between 1 and 10 nanometers and a narrow size distribution. Nanopowders are agglomerates of ultrafine particles, nanoparticles, or nanoclusters. Nanometer-sized single crystals, or single-domain ultrafine particles, are often referred to as nanocrystals.
"Ultrafine particles" (UFP) are synonymous with nanoparticles and range between 1 and 100 nm in size, as opposed to "fine particles" sized between 100 and 2,500 nm and "coarse particles" ranging from 2,500 to 10,000 nm. During the 1970s and 80s, when the first thorough fundamental studies with nanoparticles were underway in the United States (by Granqvist and Buhrman) and Japan (within an ERATO Project), researchers used the term ultrafine particles. However, during the 1990s, before the National Nanotechnology Initiative was launched in the United States, the term nanoparticle had become more common (for example, see the same senior author's paper 20 years later addressing the same issue, lognormal distribution of sizes).
The terms colloid and nanoparticle are not interchangeable. A colloid is a mixture which has solid particles dispersed in a liquid medium. The term applies only if the particles are larger than atomic dimensions but small enough to exhibit Brownian motion, with the critical size range (or particle diameter) typically ranging from nanometers (10-9 m) to micrometers (10-6 m). Colloids can contain particles too large to be nanoparticles, and nanoparticles can exist in non-colloidal form, for examples as a powder or in a solid matrix.
Although nanoparticles are associated with modern science, they have a long history. Nanoparticles were used by artisans as far back as Rome in the fourth century in the famous Lycurgus cup made of dichroic glass as well as the ninth century in Mesopotamia for creating a glittering effect on the surface of pots. In modern times, pottery from the Middle Ages and Renaissance often retains a distinct gold- or copper-colored metallic glitter. This luster is caused by a metallic film that was applied to the transparent surface of a glazing. The luster can still be visible if the film has resisted atmospheric oxidation and other weathering.
The luster originates within the film itself, which contains silver and copper nanoparticles dispersed homogeneously in the glassy matrix of the ceramic glaze. These nanoparticles are created by the artisans by adding copper and silver salts and oxides together with vinegar, ochre, and clay on the surface of previously-glazed pottery. The object is then placed into a kiln and heated to about 600 °C in a reducing atmosphere. In heat the glaze softens, causing the copper and silver ions to migrate into the outer layers of the glaze. There the reducing atmosphere reduced the ions back to metals, which then came together forming the nanoparticles that give the color and optical effects. Luster technique showed that ancient craftsmen had a sophisticated empirical knowledge of materials. The technique originated in the Muslim world. As Muslims were not allowed to use gold in artistic representations, they sought a way to create a similar effect without using real gold. The solution they found was using luster.
Michael Faraday provided the first description, in scientific terms, of the optical properties of nanometer-scale metals in his classic 1857 paper. In a subsequent paper, the author (Turner) points out that: "It is well known that when thin leaves of gold or silver are mounted upon glass and heated to a temperature that is well below a red heat (~500 °C), a remarkable change of properties takes place, whereby the continuity of the metallic film is destroyed. The result is that white light is now freely transmitted, reflection is correspondingly diminished, while the electrical resistivity is enormously increased."
Nanoparticles are of great scientific interest as they are, in effect, a bridge between bulk materials and atomic or molecular structures. A bulk material should have constant physical properties regardless of its size, but at the nano-scale, size-dependent properties are often observed. Thus, the properties of materials change as their size approaches the nanoscale and as the percentage of the surface in relation to the percentage of the volume of a material becomes significant. For bulk materials larger than one micrometer (or micron), the percentage of the surface is insignificant in relation to the volume in the bulk of the material. The interesting and sometimes unexpected properties of nanoparticles are therefore largely due to the large surface area of the material, which dominates the contributions made by the small bulk of the material.
Nanoparticles often possess unexpected physical and optical properties, as they are small enough to confine their electrons and produce quantum effects. For example, gold nanoparticles appear deep-red to black in solution. Nanoparticles of yellow gold and grey silicon are red in color. Gold nanoparticles melt at much lower temperatures (~300 °C for 2.5 nm size) than bulk gold (1064 °C);. Absorption of solar radiation is much higher in materials composed of nanoparticles than in thin films of continuous sheets of material. In both solar PV and solar thermal applications, by controlling the size, shape, and material of the particles, it is possible to control solar absorption.
Other size-dependent property changes include quantum confinement in semiconductor particles, localized surface plasmon in some metal particles and superparamagnetism in magnetic materials. Some changes in physical properties are not always desirable; for example, ferromagnetic materials smaller than 10 nm can switch their magnetisation direction using room temperature thermal energy, thus making them unsuitable for memory storage.
Suspensions of nanoparticles are possible since the interaction of the particle surface with the solvent is strong enough to overcome density differences, which otherwise usually result in a material either sinking or floating in a liquid.
The high surface area to volume ratio of nanoparticles provides a tremendous driving force for diffusion, especially at elevated temperatures. Sintering can take place at lower temperatures, over shorter time scales than for larger particles. In theory, this does not affect the density of the final product, though flow difficulties and the tendency of nanoparticles to agglomerate complicates matters. Moreover, nanoparticles have been found to impart some extra properties to various day to day products. For example, the presence of titanium dioxide nanoparticles imparts what is known as the self-cleaning effect, which lend useful water-repellant and antibacterial properties to paints and other products. Zinc oxide nanoparticles have been found to have superior UV blocking properties and are widely used in the preparation of sunscreen lotions, being completely photostable though toxic.
Clay nanoparticles when incorporated into polymer matrices increase reinforcement, leading to stronger plastics, verifiable by a higher glass transition temperature and other mechanical property tests. These nanoparticles are hard, and impart their properties to the polymer (plastic). Nanoparticles have also been attached to textile fibers in order to create smart and functionWal clothing.
Metal, dielectric, and semiconductor nanoparticles have been formed, as well as hybrid structures (e.g., core-shell nanoparticles).,  The core-shell nanoparticles can support simultaneously both electric and magnetic resonances, demoonstrating entirely new properties when compared with bare metallic nanoparticles if the resonances are properly engineered. The formation of the core-shell structure from two different metals enables an energy exchange between the core and the shell, typically found in upconverting nanoparticles and downconverting nanoparticles, and causes a shift in the emission wavelength spectrum. By introducing a dielectric layer, plasmonic core (metal)-shell (dielectric) nanoparticles enhance light absorption by increasing scattering. Recently, the metal core-dielectric shell nanoparticle has demonstrated a zero backward scattering with enhanced forward scattering on a silicon substrate when surface plasmon is located in front of a solar cell.
Nanoparticles made of semiconducting material may also be labeled quantum dots if they are small enough (typically sub 10 nm) that quantization of electronic energy levels occurs. Such nanoscale particles are used in biomedical applications as drug carriers or imaging agents with work being done to try to understand the fluid dynamic properties (e.g. drag forces) in nanoscale applications. This has shown the relationship between the fluid forces on nanoparticles and the fluid Reynolds and Knudsen numbers.
Semi-solid and soft nanoparticles have been produced. A prototype nanoparticle of semi-solid nature is the liposome. Various types of liposome nanoparticles are currently used clinically as delivery systems for anticancer drugs and vaccines.
Nanoparticles with one half hydrophilic and the other half hydrophobic are termed Janus particles and are particularly effective for stabilizing emulsions. They can self-assemble at water/oil interfaces and act as solid surfactants.
Hydrogel nanoparticles made of N-isopropylacrylamide hydrogel core shell can be dyed with affinity baits, internally. These affinity baits allow the nanoparticles to isolate and remove undesirable proteins while enhancing the target analytes.
The chemical processing and synthesis of high-performance technological components for the private, industrial, and military sectors requires the use of high-purity ceramics (oxide ceramics, such as aluminium oxide or copper(II) oxide), polymers, glass-ceramics, and composite materials, as metal carbides (SiC), nitrides (Aluminum nitrides, Silicon nitride), metals (Al, Cu), non-metals (graphite, carbon nanotubes) and layered (Al + Aluminium carbonate, Cu + C). In condensed bodies formed from fine powders, the irregular particle sizes and shapes in a typical powder often lead to non-uniform packing morphologies that result in packing density variations in the powder compact.
Uncontrolled agglomeration of powders due to attractive van der Waals forces can also give rise to microstructural heterogeneity. Differential stresses that develop as a result of non-uniform drying shrinkage are directly related to the rate at which the solvent can be removed, and thus highly dependent upon the distribution of porosity. Such stresses have been associated with a plastic-to-brittle transition in consolidated bodies, and can yield to crack propagation in the unfired body if not relieved.
In addition, any fluctuations in packing density in the compact as it is prepared for the kiln are often amplified during the sintering process, yielding inhomogeneous densification. Some pores and other structural defects associated with density variations have been shown to play a detrimental role in the sintering process by growing and thus limiting end-point densities. Differential stresses arising from inhomogeneous densification have also been shown to result in the propagation of internal cracks, thus becoming the strength-controlling flaws.
Inert gas evaporation and inert gas deposition are free many of these defects due to the distillation (cf. purification) nature of the process and having enough time to form single crystal particles, however even their non-aggreated deposits have lognormal size distribution, which is typical with nanoparticles. The reason why modern gas evaporation techniques can produce a relatively narrow size distribution is that aggregation can be avoided. However, even in this case, random residence times in the growth zone, due to the combination of drift and diffusion, result in a size distribution appearing lognormal.
It would, therefore, appear desirable to process a material in such a way that it is physically uniform with regard to the distribution of components and porosity, rather than using particle size distributions that will maximize the green density. The containment of a uniformly dispersed assembly of strongly interacting particles in suspension requires total control over interparticle forces. Monodisperse nanoparticles and colloids provide this potential. 
Monodisperse powders of colloidal silica, for example, may therefore be stabilized sufficiently to ensure a high degree of order in the colloidal crystal or polycrystalline colloidal solid that results from aggregation. The degree of order appears to be limited by the time and space allowed for longer-range correlations to be established. Such defective polycrystalline colloidal structures would appear to be the basic elements of submicrometer colloidal materials science and, therefore, provide the first step in developing a more rigorous understanding of the mechanisms involved in microstructural evolution in high performance materials and components. 
There are several methods for creating nanoparticles, including gas condensation, attrition, chemical precipitation, ion implantation, pyrolysis and hydrothermal synthesis. In attrition, macro- or micro-scale particles are ground in a ball mill, a planetary ball mill, or other size-reducing mechanism. The resulting particles are air classified to recover nanoparticles. In pyrolysis, a vaporous precursor (liquid or gas) is forced through an orifice at high pressure and burned. The resulting solid (a version of soot) is air classified to recover oxide particles from by-product gases. Traditional pyrolysis often results in aggregates and agglomerates rather than single primary particles. Ultrasonic nozzle spray pyrolysis (USP) on the other hand aids in preventing agglomerates from forming.
A thermal plasma can deliver the energy to vaporize small micrometer-size particles. The thermal plasma temperatures are in the order of 10,000 K, so that solid powder easily evaporates. Nanoparticles are formed upon cooling while exiting the plasma region. The main types of the thermal plasma torches used to produce nanoparticles are dc plasma jet, dc arc plasma, and radio frequency (RF) induction plasmas. In the arc plasma reactors, the energy necessary for evaporation and reaction is provided by an electric arc formed between the anode and the cathode. For example, silica sand can be vaporized with an arc plasma at atmospheric pressure, or thin aluminum wires can be vaporized by exploding wire method. The resulting mixture of plasma gas and silica vapour can be rapidly cooled by quenching with oxygen, thus ensuring the quality of the fumed silica produced.
In RF induction plasma torches, energy coupling to the plasma is accomplished through the electromagnetic field generated by the induction coil. The plasma gas does not come in contact with electrodes, thus eliminating possible sources of contamination and allowing the operation of such plasma torches with a wide range of gases including inert, reducing, oxidizing, and other corrosive atmospheres. The working frequency is typically between 200 kHz and 40 MHz. Laboratory units run at power levels in the order of 30-50 kW, whereas the large-scale industrial units have been tested at power levels up to 1 MW. As the residence time of the injected feed droplets in the plasma is very short, it is important that the droplet sizes are small enough in order to obtain complete evaporation. The RF plasma method has been used to synthesize different nanoparticle materials, for example synthesis of various ceramic nanoparticles such as oxides, carbours/carbides, and nitrides of Ti and Si (see Induction plasma technology).
Inert-gas condensation is frequently used to produce metallic nanoparticles. The metal is evaporated in a vacuum chamber containing a reduced atmosphere of an inert gas. Condensation of the supersaturated metal vapor results in creation of nanometer-size particles, which can be entrained in the inert gas stream and deposited on a substrate or studied in situ. Early studies were based on thermal evaporation. Using magnetron sputtering to create the metal vapor allows to achieve higher yields. The method can easily be generalized to alloy nanoparticles by choosing appropriate metallic targets. The use of sequential growth schemes, where the particles travel through a second metallic vapor, results in growth of core-shell (CS) structures.
Nanoparticles can also be formed using radiation chemistry. Radiolysis from gamma rays can create strongly active free radicals in solution. This relatively simple technique uses a minimum number of chemicals. These including water, a soluble metallic salt, a radical scavenger (often a secondary alcohol), and a surfactant (organic capping agent). High gamma doses on the order of 104Gray are required. In this process, reducing radicals will drop metallic ions down to the zero-valence state. A scavenger chemical will preferentially interact with oxidizing radicals to prevent the re-oxidation of the metal. Once in the zero-valence state, metal atoms begin to coalesce into particles. A chemical surfactant surrounds the particle during formation and regulates its growth. In sufficient concentrations, the surfactant molecules stay attached to the particle. This prevents it from dissociating or forming clusters with other particles. Formation of nanoparticles using the radiolysis method allows for tailoring of particle size and shape by adjusting precursor concentrations and gamma dose.
The sol-gel process is a wet-chemical technique (also known as chemical solution deposition) widely used recently in the fields of materials science and ceramic engineering. Such methods are used primarily for the fabrication of materials (typically a metal oxide) starting from a chemical solution (sol, short for solution), which acts as the precursor for an integrated network (or gel) of either discrete particles or network polymers. 
Typical precursors are metal alkoxides and metal chlorides, which undergo hydrolysis and polycondensation reactions to form either a network "elastic solid" or a colloidal suspension (or dispersion) - a system composed of discrete (often amorphous) submicrometer particles dispersed to various degrees in a host fluid. Formation of a metal oxide involves connecting the metal centers with oxo (M-O-M) or hydroxo (M-OH-M) bridges, therefore generating metal-oxo or metal-hydroxo polymers in solution. Thus, the sol evolves toward the formation of a gel-like diphasic system containing both a liquid phase and solid phase whose morphologies range from discrete particles to continuous polymer networks.
In the case of the colloid, the volume fraction of particles (or particle density) may be so low that a significant amount of fluid may need to be removed initially for the gel-like properties to be recognized. This can be accomplished in a number of ways. The most simple method is to allow time for sedimentation to occur, and then pour off the remaining liquid. Centrifugation can also be used to accelerate the process of phase separation.
Removal of the remaining liquid (solvent) phase requires a drying process, which typically causes shrinkage and densification. The rate at which the solvent can be removed is ultimately determined by the distribution of porosity in the gel. The ultimate microstructure of the final component will clearly be strongly influenced by changes implemented during this phase of processing. Afterward, a thermal treatment, or firing process, is often necessary in order to favor further polycondensation and enhance mechanical properties and structural stability via final sintering, densification, and grain growth. One of the distinct advantages of using this methodology as opposed to the more traditional processing techniques is that densification is often achieved at a much lower temperature.
The precursor sol can be either deposited on a substrate to form a film (e.g., by dip-coating or spin-coating), cast into a suitable container with the desired shape (e.g., to obtain a monolithic ceramics, glasses, fibers, membranes, aerogels), or used to synthesize powders (e.g., microspheres, nanospheres). The sol-gel approach is a cheap and low-temperature technique that allows for the fine control of the product's chemical composition. Even small quantities of dopants, such as organic dyes and rare earth metals, can be introduced in the sol and end up uniformly dispersed in the final product. It can be used in ceramics processing and manufacturing as an investment casting material, or as a means of producing very thin films of metal oxides for various purposes. Sol-gel derived materials have diverse applications in optics, electronics, energy, space, (bio)sensors, medicine (e.g., controlled drug release) and separation (e.g., chromatography) technology.
Ion implantation may be used to treat the surfaces of dielectric materials such as sapphire and silica to make composites with near-surface dispersions of metal or oxide nanoparticles. See ion implantation#Ion implantation-induced nanoparticle formation
Scientists have taken to naming their particles after the real-world shapes that they might represent. Nanospheres,nanorods, nanochains, nanoreefs, nanoboxes and more have appeared in the literature. These morphologies sometimes arise spontaneously as an effect of a templating or directing agent present in the synthesis such as miscellar emulsions or anodized alumina pores, or from the innate crystallographic growth patterns of the materials themselves. Some of these morphologies may serve a purpose, such as long carbon nanotubes used to bridge an electrical junction, or just a scientific curiosity like the stars shown at right.
Amorphous particles usually adopt a spherical shape (due to their microstructural isotropy), whereas the shape of anisotropic microcrystalline whiskers corresponds to their particular crystal habit. At the small end of the size range, nanoparticles are often referred to as clusters. Spheres, rods, fibers, and cups are just a few of the shapes that have been grown. The study of fine particles is called micromeritics.
Nanoparticles have different analytical requirements than conventional chemicals, for which chemical composition and concentration are sufficient metrics. Nanoparticles have other physical properties that must be measured for a complete description, such as size, shape, surface properties, crystallinity, and dispersion state. Additionally, sampling and laboratory procedures can perturb their dispersion state or bias the distribution of other properties. In environmental contexts, an additional challenge is that many methods cannot detect low concentrations of nanoparticles that may still have an adverse effect. For some applications, nanoparticles may be characterized in complex matrices such as water, soil, food, polymers, inks, complex mixtures of organic liquids such as in cosmetics, or blood.
There are several overall categories of methods used to characterize nanoparticles. Microscopy methods generate images of individual nanoparticles to characterize their shape, size, and location. Electron microscopy and scanning probe microscopy are the dominant methods. Because nanoparticles have a size below the diffraction limit of visible light, conventional optical microscopy is not useful. Electron microscopes can be coupled to spectroscopic methods that can perform elemental analysis. Microscopy methods are destructive, and can be prone to undesirable artifacts from sample preparation, or from probe tip geometry in the case of scanning probe microscopy. Additionally, microscopy is based on single-particle measurements, meaning that large numbers of individual particles must be characterized to estimate their bulk properties.
Spectroscopy, which measures the particles' interaction with electromagnetic radiation as a function of wavelength, is useful for some classes of nanoparticles to characterize concentration, size, and shape. X-ray, ultraviolet-visible, infrared, and nuclear magnetic resonance spectroscopy can be used with nanoparticles.Light scattering methods using laser light, X-rays, or neutron scattering are used to determine particle size, with each method suitable for different size ranges and particle compositions. Some miscellaneous methods are electrophoresis for surface charge, the Brunauer-Emmett-Teller method for surface area, and X-ray diffraction for crystal structure, as well as mass spectrometry for particle mass, and particle counters for particle number.Chromatography, centrifugation, and filtration techniques can be used to separate nanoparticles by size or other physical properties before or during characterization.
Functionalization is the introduction of organic molecules or polymers on the surface of the nanoparticle. The surface coating of nanoparticles determines many of their physical and chemical properties, notably stability, solubility, and targeting. A coating that is multivalent or polymeric confers high stability. Functionalized nanomaterial-based catalysts can be used for catalysis of many known organic reactions.
An environmentally friendly and facile functionalization approach for synthesizing highly dispersed Graphene was developed. In this approach, graphenes were functionalized covalently with Gallic Acid (GA) in a one-pot free radical grafting method. This cost-effective method could be used for industrial mass production. The suspension of Gallic acid-functionalized graphene in water was test as a high performance heat transfer fluids for improved convective heat transfer in closed conduit flows.
For biological applications, the surface coating should be polar to give high aqueous solubility and prevent nanoparticle aggregation. In serum or on the cell surface, highly charged coatings promote non-specific binding, whereas polyethylene glycol linked to terminal hydroxyl or methoxy groups repel non-specific interactions. Nanoparticles can be linked to biological molecules that can act as address tags, to direct the nanoparticles to specific sites within the body, specific organelles within the cell, or to follow specifically the movement of individual protein or RNA molecules in living cells. Common address tags are monoclonal antibodies, aptamers, streptavidin or peptides. These targeting agents should ideally be covalently linked to the nanoparticle and should be present in a controlled number per nanoparticle. Multivalent nanoparticles, bearing multiple targeting groups, can cluster receptors, which can activate cellular signaling pathways, and give stronger anchoring. Monovalent nanoparticles, bearing a single binding site, avoid clustering and so are preferable for tracking the behavior of individual proteins.
Red blood cell coatings can help nanoparticles evade the immune system.
Nanoparticles present possible dangers, both medically and environmentally. Most of these are due to the high surface to volume ratio, which can make the particles very reactive or catalytic. They are also able to pass through cell membranes in organisms, and their interactions with biological systems are relatively unknown. However, it is unlikely the particles would enter the cell nucleus, Golgi complex, endoplasmic reticulum or other internal cellular components due to the particle size and intercellular agglomeration. A recent study looking at the effects of ZnO nanoparticles on human immune cells has found varying levels of susceptibility to cytotoxicity. There are concerns that pharmaceutical companies, seeking regulatory approval for nano-reformulations of existing medicines, are relying on safety data produced during clinical studies of the earlier, pre-reformulation version of the medicine. This could result in regulatory bodies, such as the FDA, missing new side effects that are specific to the nano-reformulation. However considerable research has demonstrated that zinc nanoparticles are not absorbed into the bloodstream in vivo.
Concern has also been raised over the health effects of respirable nanoparticles from certain combustion processes. As of 2013 the U.S. Environmental Protection Agency was investigating the safety of the following nanoparticles:
As of 2016, the U.S. Environmental Protection Agency had conditionally registered, for a period of four years, only two nanomaterial pesticides as ingredients. The EPA differentiates nanoscale ingredients from non-nanoscale forms of the ingredient, but there is little scientific data about potential variation in toxicity. Testing protocols still need to be developed.
As the most prevalent morphology of nanomaterials used in consumer products, nanoparticles have potential and actual applications in all industries. Table below summarizes the most common nanoparticles used in various product types available on the global markets.
|1||agriculture||silver, silicon dioxide, potassium, calcium, iron, zinc, phosphorus, boron, zinc oxide and molybdenum|
|2||automotive||tungsten, disulfidesilicon dioxide, clay, titanium dioxide, diamond, copper, cobalt oxide, zinc oxide, boron nitride, zirconium dioxide, tungsten, ?-aluminium oxide, boron, palladium, platinum, cerium(IV) oxide, carnauba, aluminium oxide, silver, calcium carbonate and calcium sulfonate|
|3||construction||titanium, dioxidesilicon dioxide, silver, clay, aluminium oxide, calcium carbonate calcium silicate hydrate, carbon, aluminium phosphate cerium(IV) oxide and calcium hydroxide|
|4||cosmetics||silver, titanium dioxide, gold, carbon, zinc oxide, silicon dioxide, clay, sodium silicate, kojic acid and hydroxy acid|
|5||electronics||silver, aluminum, silicon dioxide and palladium|
|6||environment||silver, titanium dioxide, carbonmanganese oxide, clay, gold and selenium|
|7||food||silver, clay, titanium dioxide, gold, zinc oxide, silicon dioxide, calcium, copper, zinc, platinum, manganese, palladium and carbon|
|8||home appliance||silver, zinc oxide, silicon dioxide, diamond and titanium dioxide|
|9||medicine||silver, gold, hydroxyapatite, clay, titanium dioxide, silicon dioxide, zirconium dioxide, carbon, diamond, aluminium oxide and ytterbium trifluoride|
|10||petroleum||tungsten, disulfidezinc oxide, silicon dioxide, diamond, clay, boron, boron nitride, silver, titanium dioxide, tungsten, ?-aluminium oxide, carbon, molybdenum disulfide and ?-aluminium oxide|
|11||printing||toner, deposited by a printer onto paper or other substrate|
|12||renewable energies||titanium, palladium, tungsten disulfide, silicon dioxide, clay, graphite, zirconium(IV) oxide-yttria stabilized, carbon, gd-doped-cerium(IV) oxide, nickel cobalt oxide, nickel(II) oxide, rhodium, sm-doped-cerium(IV) oxide, barium strontium titanate and silver|
|13||sports and fitness||silver, titanium dioxide, gold, clay and carbon|
|14||textile||silver, carbon, titanium dioxide, copper sulfide, clay, gold, polyethylene terephthalate and silicon dioxide|
Scientific research on nanoparticles is intense as they have many potential applications in medicine, physics, optics, and electronics. The U.S. National Nanotechnology Initiative offers government funding focused on nanoparticle research.|The use of nanoparticles in laser dye-doped poly(methyl methacrylate) (PMMA) laser gain media was demonstrated in 2003 and it has been shown to improve conversion efficiencies and to decrease laser beam divergence. Researchers attribute the reduction in beam divergence to improved dn/dT characteristics of the organic-inorganic dye-doped nanocomposite. The optimum composition reported by these researchers is 30% w/w of SiO2 (~ 12 nm) in dye-doped PMMA.|Nanoparticles are being investigated as potential drug delivery system. Drugs, growth factors or other biomolecules can be conjugated to nano particles to aid targeted delivery. This nanoparticle-assisted delivery allows for spatial and temporal controls of the loaded drugs to achieve the most desirable biological outcome. Nanoparticles are also studied for possible applications as dietary supplements for delivery of biologically active substances, for example mineral elements.